Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript

International Journal of Solids and Structures 40 (2003) 2611–2643 www.elsevier.com/locate/ijsolstr On the coupling of anisotropic damage and plasticity models for ductile materials Rashid K. Abu Al-Rub, George Z. Voyiadjis * Department of Civil and Environmental Engineering, Louisiana State University, CEBA 3508-B, Baton Rouge, LA 70803, USA Received 11 February 2003; received in revised form 11 February 2003 Abstract In this contribution various aspects of an anisotropic damage model coupled to plasticity are considered. The model is formulated within the thermodynamic framework and implements a strong coupling between plasticity and damage. The constitutive equations for the damaged material are written according to the principle of strain energy equivalence between the virgin material and the damaged material. The damaged material is modeled using the constitutive laws of the eﬀective undamaged material in which the nominal stresses are replaced by the eﬀective stresses. The model considers diﬀerent interaction mechanisms between damage and plasticity defects in such a way that two-isotropic and twokinematic hardening evolution equations are derived, one of each for the plasticity and the other for the damage. An additive decomposition of the total strain into elastic and inelastic parts is adopted in this work. The elastic part is further decomposed into two portions, one is due to the elastic distortion of the material grains and the other is due to the crack closure and void contraction. The inelastic part is also decomposed into two portions, one is due to nucleation and propagation of dislocations and the other is due to the lack of crack closure and void contraction. Uniaxial tension tests with unloadings have been used to investigate the damage growth in high strength steel. A good agreement between the experimental results and the model is obtained. Ó 2003 Elsevier Science Ltd. All rights reserved. Keywords: Anisotropic damage; Damage mechanics; Plasticity; Thermodynamics; Isotropic hardening; Kinematic hardening 1. Introduction The non-linear material behavior may be attributed to two distinct material mechanical processes: plasticity (i.e. dislocations along crystal slip planes) and damage mechanics (microcracks, microcavities nucleation and coalescence, decohesions, grain boundary cracks, and cleavage in regions of high stress concentration). The two degradation phenomena are described best by the theories of plasticity and continuum damage mechanics. Thus, a multi-dissipative model that accounts for both the material decohesions and the dislocations along slip planes is necessary. This is accomplished by adopting two loading surfaces and two potential functions, one for plasticity and the other for damage. * Corresponding author. Tel.: +1-225-578-8668; fax: +1-225-578-9176. E-mail address: [email protected] (G.Z. Voyiadjis). 0020-7683/03/$ - see front matter Ó 2003 Elsevier Science Ltd. All rights reserved. doi:10.1016/S0020-7683(03)00109-4 2612 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 Ductile materials usually fail as the result of nucleation, growth, and coalescence of microdamages. Experimental observations show that the accumulation of microdamages has a tendency to form macroscopically localized damage, which is a precursor to failure. This progressive physical process of degradation of the material mechanical properties up to complete failure is commonly referred to as damage. Various damage morphologies have been described in the literature, such as creep damage, low cycle fatigue, high cycle fatigue, and brittle damage (Kachanov, 1986; Lemaitre and Chaboche, 1990; Lemaitre, 1992; Voyiadjis and Kattan, 1999). The present paper is concerned with anisotropic ductile damage. Metallographic studies for polycrystalline metals (Thomason, 1990; Anderson, 1994; Hertzberg, 1996) demonstrate that the ductile damage is basically characterized by three mechanisms of microdamages growth: (i) nucleation of microscopic voids that initiate at inclusions and second phase particles, failure of particles or microcracking of the matrix surrounding the inclusion, (ii) growth of the microvoids by means of plastic strain and hydrostatic stress, and (iii) coalescence or microcracks linking the growing microvoids with adjacent ones, thus leading to vanishing load carrying capacity of the material, as the damage density approaches unity. Many models for estimating the microdamage accumulation in ductile materials have been published, some of which are based on damage micromechanics (micromechanical damage models) while others based on the continuum damage theory (phenomenological damage models). The former models are required for particles of less than 1 lm in diameter. A model of this type was formulated by Gurson (1977), where he obtained, based on an approximation analysis of spherical voids, a yield function for porous ductile materials with perfectly plastic matrix. Modiﬁcation of the GursonÕs model have been proposed by several authors (e.g. Tvergaard, 1982; Tvergaard and Needleman, 1984). Tvergaard (1982) modiﬁed GursonÕs model to improve the predictions at low void volume fractions. Tvergaard and Needleman (1984) modiﬁed GursonÕs yield function in order to account for rate sensitivity and necking instabilities in plastically deforming solids and to provide better representation of ﬁnal void coalescence. The aspects of GursonÕs model was outlined in the review article by Nemat-Nasser (1992) and discussed by Voyiadjis and Kattan (1992a,b), Li (2000), and Mahnken (2002). In this way micromechanical models are based on physical soundness, and various applications have modeled microdamage growth and ductile failure (Haj-Ali et al., 2001). Phenomenological models are based on the concept of Kachanov (1958), who was the ﬁrst to introduce for the isotropic case a one-dimensional variable, which may be interpreted as the eﬀective surface density of microdamages per unit volume (Voyiadjis and Venson, 1995; Venson and Voyiadjis, 2001). Kachanov (1958) pioneered the subject of continuum damage mechanics by introducing the concept of eﬀective stress. This concept is based on considering a ﬁctitious undamaged conﬁguration of a body and comparing it with the actual damaged conﬁguration. He originally formulated his theory using simple uniaxial tension. Following KachanovÕs work researchers in diﬀerent ﬁelds applied continuum damage mechanics to their areas in ﬁelds like brittle materials (Krajcinovic and Foneska, 1981; Krajcinovic, 1983, 1996) and ductile materials (Lemaitre, 1984, 1985; Kachanov, 1986; Murakami, 1988). In the 1990s applications of continuum damage mechanics to plasticity have appeared (e.g. Lubarda and Krajcinovic, 1995; Voyiadjis and Kattan, 1992a,b, 1999; Voyiadjis and Park, 1997, 1999; Voyiadjis and Deliktas, 2000; etc.). Often, ductile materials undergo a strong plastic deformation, which has a major inﬂuence on the damage evolution and reverse. There are many models with weak coupling between plasticity and damage. The models that adopt two separate uncoupled damage and plastic loading surfaces with two independent associated ﬂow rules present a week coupling between plasticity and damage. Those models are being extensively used by many authors (e.g. Chow and Wang, 1987, 1988; Simo and Ju, 1989; Lemaitre and Chaboche, 1990; Hansen and Schreyer, 1994; Zhu and Cescetto, 1995; Murakami et al., 1998; etc.). While there are many models with weak coupling, no consistent model realizing a strong coupling has been published yet. However, relatively strong coupling between plasticity and damage can be achieved by using one single smooth generalized yield surface and an associated ﬂow rule for the plasticity and damage R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2613 evolutions (e.g. Gurson, 1977; Tvergaard, 1982; Tvergaard and Needleman, 1984; Rousselier, 1987; Ehlers, 1995; Hesebeck, 2001; Mahnken, 2002). Those models obviously cannot describe all loadings correctly since a hydrostatic stress will certainly cause damage before any plastic deformation can be noticed. In addition most of those models are restricted to low damage levels or dilute distribution of defects and therefore they fail to account for the interaction of the defects adequately. Another approach to achieve this strong coupling is by using separate plasticity and damage surfaces with separate non-associated ﬂow rules in such a way that both damage and plasticity ﬂow rules are dependent on both the plastic and damage potentials (Voyiadjis and Deliktas, 2000). The later approach is adopted in this work, where the strong coupling between plasticity and damage is implemented by using two damage mechanisms. One mechanism is coupled with plasticity, while the other one occurs independent of plastic deformation. The dissipation function of the latter occurs in both the elastic and plastic domains. To formulate that on the basis of the thermodynamic principles, the two damage processes are represented by two additive portions in the dissipation potentials. Because this work focuses on the development of coupled plastic-damage governing equations based on thermomechanical postulates, the various possibilities to describe the plasticity and anisotropic damage shall be considered here. It is generally assumed that the rate of deformation can be additively decomposed into an elastic (reversible) part and an inelastic (irreversible) part (e.g. Nemat-Nasser, 1983; Lubliner, 1990; Simo and Hughes, 1998). ÔNon-instantaneously reversibleÕ deformation is a more general description of the inelastic deformation since it is corresponding to the following set of physical phenomena: instantaneous plasticity, viscoplasticity, damage, and viscodamage. The ﬁrst type of inelastic deformation is a time-independent mechanism, which is generally considered in the rate-independent plasticity theories. The viscoplastic deformation, which is sometimes qualiﬁed as creep, is a rate-dependent mechanism. Both of those two mechanisms or one of them is generally not suﬃcient to describe the set of experimental observations. Therefore, degradation of the mechanical properties up to complete failure should be considered in the experimental simulations. The damage growth can be time-independent (damage theory) and/or timedependent process (viscodamage theory). The evolution, nucleation, and coalescence of microcracks, voids, and cavities during manufacturing processes and subsequent loading enhance the material to behave inelastically in the elastic and plastic domains. Voyiadjis and Park (1999) summed such defects as an inelastic strain called the damage strain. They decomposed this damage strain into elastic-damage (recoverable) component attributed to crack closure and void contraction during unloading, and inelastic-damage (unrecoverable) component attributed to random distribution and orientation of the cracks that make their recovery impossible. In accordance with their work, two irreversible strains are considered in this study: the plastic and the damage strains. An outline for this work is as follows: In Section 2 we demonstrate the motivated morphologies for the additive decomposition of the total strain into elastic, plastic, and damage components. Section 3 is devoted to the physical interpretations of the damage variable for both the isotropic and anisotropic damage distributions. Furthermore the derivation of the energy release rate is outlined for both isotropic and anisotropic damage distributions. In Section 4, we outline a general thermodynamic framework for the coupled elasto-plastic and damage material behavior. In Section 5, the derived evolution equations are examined for pure isotropic damage case and applied to simulate the experimental results of Hesebeck (2001) for high strength steel specimens subjected to tensile loading. This work is restricted to small strains. 2. The strain additive decomposition Experimental observations show that in general the processes of cold-working, forming, machining of mechanical parts, etc. can cause an initial evolution of defects in the virgin material state, such as nucleation of certain amount of cracks, voids, and dislocation patterns. The initial defects induced in the material 2614 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 microstructure along with the subsequent defects that occur during deformation process enhance the material to behave inelastically even before the onset of plasticity. If the material is elastically unloaded before forming dislocations along slip planes (plasticity), permanent strains are observed. Those strains are irreversible damage strains, while the reversible strains are of two parts: elastic part and damage part. As plastic deformations initiate, both damage and plastic permanent deformations are anticipated. Next we demonstrate this behavior in uniaxial tension and complex loadings. Imagine an elastically loaded representative volume element (RVE) containing uniformly distributed (micro)cracks of Mode I, which are triggered by the process of cold working, is deformed by a total strain e1 . A certain part of this strain is elastically recoverable (ee1 ) and another part is induced by damage (eed 1 ). After the loads are released before the yield limit is reached, the body will have no permanent strains left. However, the magnitude of the elastic stiﬀness for the RVE maybe reduced due to the growth of microcracks. This is clearly demonstrated in Fig. 1 which shows the foregoing micromechanics of a continuum point in the RVE and the corresponding macrostresses and strains. We begin with an unstressed unit cell in the RVE containing a microcrack of length 2a and a resulting average stiﬀness E1 (the stiﬀness of the matrix surrounding the microcrack remains unchanged by microcrack opening). Up to a certain stress level, the microcrack will not grow but only open. Therefore, the microcrack length will remain 2a (neglecting the PoissonÕs eﬀect) and the RVE average stiﬀness will not change. Beyond this threshold, however, the microcrack extends by an amount 2ðdaÞ and the average stiﬀness decreases by an amount dE1 . Upon the load release the microcrack will close and no further growth occurs. For the same stress (points b and d) a greater strain will result, due to the reduction in the RVE average stiﬀness. In the stress free state there are no permanent strains left, only the resulted average stiﬀness (E1 ) is less than that of the initial body. The amount of the stored elastic strain energy at the end of the loading process is given by r1c ðee1c þ eed 1c Þ=2 and the additional surface energy resulting from the microcrack extension by an amount of 2da is obtained from e e the work done by the applied stress r1c ½ðee1c þ eed 1c Þ ðe1a þ e1a Þ. Imagine now the elastically loaded RVE containing an arbitrary distribution of (micro)voids and (micro)cracks of mixed modes (Mode I, II, and III), which are triggered by the process of cold working, and subjected to a 2-D state of stress. Generally, this situation is more likely to happen in materials than the Fig. 1. Fictitious uniaxial stress–strain elastic response resulting from a growing microcrack. All the damage strain is recoverable (the crack is closed but not healed). R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2615 former case. The RVE is deformed by a total strain of e; a certain part of it is elastically recoverable (ee ) and another part is induced by the damage (ed ). When the loads are released before yielding is observed, the body will have, similar to plasticity and in contrast to the previous ﬁctitious situation, permanent deformations (eid ). Those irreversible damage strains are attributed to the necessary geometric constraints set by other (micro)defects. Fig. 2 shows the underlying micromechanics of a continuum point in the RVE and the corresponding macrostresses and strains in one of the geometric directions. The existing stress state is assumed of combined biaxial tension and shear (r2 > r1 > s12 ) with the stress–strain behavior in the twodirection being accounted for. We start with an unstressed sub-RVE containing a growing microcrack and microvoid with an average stiﬀness E (the stiﬀness of the matrix surrounding the microcrack/microvoid remains unchanged by microcrack opening). Up to a certain stress level, the microcrack will open and start growing and the microvoid will expand. This process is accompanied by shape change and reduction in the average stiﬀness, dE. Upon the loads release, part of the microcrack will close, the size of the microvoid will decrease, and no further growth occurs. For the same stress (points b and d) a greater strain will result, due to the microcrack and microvoid growth and the reduction in the average stiﬀness. In the stress free state, permanent strains occur and the resulted average stiﬀness (E) is less than that of the initial body. Part of the resulted damage strain, ed , is recovered and another part is permanent. As clearly seen, the recoverable part, eed , is attributed to partial closure of microcracks and size reduction of microvoids upon unloading (but not healing), while the unrecoverable part is attributed to lack of closure of all microcracks and unvanishing microvoids that cause permanent deformation. As we stated earlier, this may be due to the geometrical constraints set up by the interacting microcracks, microvoids, and grain boundaries. Both situations are likely to happen under diﬀerent types of loading. However, the ﬁrst situation is more likely to happen in uniaxial tension, while the second situation is likely to happen in complex loading. One now investigates the total basic one-dimensional behavior in a ductile material. Consider the uniaxial tension test shown in Fig. 3. In this test, a bar of uniform cross-section is subjected to the uniaxial loading–unloading history: O ! B ! C, during which the length of the bar takes the following values: L ! lp ! lpid ! lpd ! l. Stage O ! B corresponds to a monotonic loading beyond the elasticity domain, Fig. 2. Fictitious stress–strain elastic response of an RVE subjected to a 2-D state of stress (r1 > r2 > s12 ) resulting from a growing microcrack and microvoid. Part of the damage strain is recoverable (not healed) and the other part is unrecoverable. 2616 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 Fig. 3. Uniaxial stress–strain response of a metallic specimen. and B ! C to elastic unloading (C ! B corresponds to elastic loading process). State C corresponds to a stress-free, unloaded conﬁguration. We can write the following identity: l l lpd lp ¼ pd p L l l L ð1Þ k ¼ ke kd kp ð2Þ or where k ¼ l=L is the axial stretch ratio at the end of O ! B, ke ¼ l=lpd can be viewed as the elastic stretch at the end of the elastic transformation B ! F, kd ¼ lpd =lp corresponds to the damage stretch between D state and a damage-free state between C and O, and kp ¼ lp =L corresponds to plastic stretch between O state and a plastic-free state between C and O. The term ‘‘between C and O’’ is used due to the fact that part of the permanent deformation is contributed by plasticity and part from the non-recoverable damage. Note that the superscripts here do not imply tensorial indices but merely indicate the corresponding deformation conﬁguration such as ‘‘e’’ for elastic, ‘‘p’’ for plastic, ‘‘d’’ for damage, ‘‘ed’’ for elastic-damage, ‘‘id’’ for inelastic-damage, and ‘‘pid’’ for plastic-inelastic-damage Additionally kd can be written as: lpd lpd lpid ¼ pid p lp l l ð3Þ kd ¼ ked kid ð4Þ or ed where k ¼ lpd =lpid is the elastic-damage stretch (recoverable damage stretch) between states D ! C, and kid ¼ lpid =lp is the unrecoverable damage stretch between C state and a damage-free state between C and O. No eﬀective conﬁgurations are used to interpret the above deﬁnitions. In the context of the kinematic linear theory of deformation (inﬁnitesimal deformation) and motivated by the above schematic illustration, by the micromechanics of single crystal plasticity (Nemat-Nasser, 1979, 1983), and the continuum damage mechanics (Voyiadjis and Park, 1999), one can assume the additive R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2617 decomposition of the total strain (e) into elastic (ee ), plastic (ep ), and damage components (ed ). Although the damage process is an irreversible deformation thermodynamically; however, the deformation due to damage itself can be partially or completely recovered upon unloading. Thus, the damage strain component is also decomposed into elastic (reversible) and inelastic (irreversible) parts. The recoverable part is attributed to cracks closure upon unloading (but not healing), while the unrecoverable part is attributed to unclosed cracks and voids that cause permanent deformation. This may be due to the constraints set up by the interacting (micro)cracks, (micro)voids, dislocation densities, and grain boundaries. Both reversible and irreversible parts cause degradation in the material stiﬀness. Hence, in small strain theory, the total strain can be additively decomposed as: eij ¼ eeij þ epij þ edij ð5Þ id edij ¼ eed ij þ eij ð6Þ and where eed and eid are the elastic-damage and inelastic-damage parts of the damage strain, respectively. In this work the subscripted letters after the variables indicate the tensorial nature of the variables unless speciﬁcally stated otherwise. During the unloading process, two types of strains are purely reversible: the ordinary elastic strain, ee , and the elastic-damage strain, eed . Thus, the total reversible elastic strain, eE , due to unloading can be obtained by: eEij ¼ eeij þ eed ij ð7Þ On the other hand, the total inelastic strain, eI , arises from the two irreversible sources: inelastic damage and plastic ﬂow such that: p eIij ¼ eid ij þ eij ð8Þ Eq. (5) can therefore be expressed as follows: eij ¼ eEij þ eIij ð9Þ Both components of the damage tensor eed and eid are functions of an internal variable called the damage variable, /, which is a scalar for isotropic damage and a tensor for a continuum that exhibits anisotropic damage. In the following section, we interpret the physical deﬁnition of the damage tensor in one-dimension and three-dimensions. 3. Physical interpretation of the damage variable The damage variable is a macroscopic measure of the microscopic degradation of a RVE (Kachanov, 1986; Lemaitre and Chaboche, 1990; Lemaitre, 1992; Lubarda and Krajcinovic, 1993; Voyiadjis and Venson, 1995; Krajcinovic, 1996; Voyiadjis and Kattan, 1999; Voyiadjis and Deliktas, 2000). Damage in materials can be represented in many forms such as speciﬁc void and crack surfaces, speciﬁc crack and void volumes, the spacing between cracks or voids, scalar representation of damage, and general tensorial representation of damage. In this section, however, the physical interpretation of the damage variable is introduced as the speciﬁc damaged surface area, where two cases are considered: the isotropic damage distribution case and the anisotropic damage distribution case of microcracks and microvoids. Moreover, this study is limited to small strain deformations and an extension to ﬁnite strain deformations can be easily done. 2618 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 3.1. Isotropic damage We ﬁrst consider the deﬁnition of the damage variable / in one-dimension as originally proposed by Kachanov (1958), and further developed by several other authors (e.g. Lemaitre and Chaboche, 1990; Lemaitre, 1992; Lubarda and Krajcinovic, 1993; Voyiadjis and Venson, 1995; Krajcinovic, 1996; Voyiadjis and Kattan, 1999; Kattan and Voyiadjis, 2001) since the 1970s. Consider a uniform bar subjected to a uniaxial tensile load, T , as shown in Fig. 4(a). The cross-sectional area of the bar in the stressed conﬁguration is A and it is assumed that both voids and cracks appear as damage in the bar and form a total damage area of AD . The uniaxial tensile force T acting on the bar is easily expressed using the formula T ¼ rA. In order to use the principles of continuum damage mechanics, one considers a ﬁctitious undamaged conﬁguration (eﬀective conﬁguration) of the bar as shown in Fig. 4(b). In this conﬁguration all types of damage, including both voids and cracks, are removed from the bar. The eﬀective stressed crosssectional area of the bar in this conﬁguration is denoted by A and the eﬀective uniaxial stress is r. The bars in both the damaged conﬁguration and the eﬀective undamaged conﬁguration are subjected to the same tensile force, T . Therefore, considering the eﬀective undamaged conﬁguration, one can write T ¼ rA. Equating the two expressions for T that are obtained from both conﬁgurations, the following expression for the eﬀective uniaxial stress r (Kachanov, 1958; Rabotnov, 1968) is derived such that: r ð10Þ r¼ 1/ where /¼ A A AD ¼ A A ð11Þ where AD is the speciﬁc ﬂaws (or damaged) area (Voyiadjis and Kattan, 1999; Kattan and Voyiadjis, 2001). Similarly, a relation between the eﬀective stress tensor, r, and the nominal stress tensor, r, for the case of isotropic damage (i.e. scalar damage variable) can be written as follows: rij ð12Þ rij ¼ 1/ One can now derive expressions for the elastic strains and elastic moduli in the damage conﬁguration as a function of the isotropic damage variable /. Assume that the initiated microcracks (no microvoids are Fig. 4. A cylindrical bar subjected to uniaxial tension: both voids and cracks are removed simultaneously (Voyiadjis and Kattan, 1999; Kattan and Voyiadjis, 2001). R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2619 initiated) during elastic loading are totally closed (not healed) upon elastic unloading process. Fig. 5(a) shows a ﬁctitious stress–strain response before plasticity occurs, where the total elastic strain (eE ¼ ee þ eed ) is recoverable. Thus, the elastic stress–strain relation can be written as: rij ¼ Eijkl eekl ð13Þ where E is the initial elastic moduli that is constant and can be obtained experimentally. The above equation shows that the initial elastic modulus, E, is equal to the eﬀective elastic modulus, E, if no damage occurs (i.e. E ¼ E for no damage case). This is true if initially the current state has no microdamage initiation. Thus, in this case the spatial conﬁguration coincides with the eﬀective ﬁctitious conﬁguration. Alternatively, Eq. (13) can also be written as follows (Fig. 5(a)): E rij ¼ Eijkl ðeekl þ eed kl Þ ¼ Eijkl ekl ð14Þ where E is the elastic-damage YoungÕs moduli (degraded) that is no longer constant, and hence a relation between the elastic-damage moduli E and the damage variable / is sought. Considering the ﬁctitious eﬀective (undamaged) stress–strain response shown in Fig. 5(b), a similar relation to Eq. (13) can be obtained such as: rij ¼ Eijkl eekl ð15Þ where ee and E are the eﬀective counterparts of eE and E, respectively. In order to derive the transformation relations between the damaged and the hypothetical undamaged (eﬀective conﬁguration) states of the material, the elastic energy equivalence hypothesis (Sidoroﬀ, 1981) is utilized. This hypothesis assumes that the elastic energy in terms of eﬀective and nominal stress and corresponding strain quantities must be equal. Thus, the elastic strain energy is equated to the eﬀective elastic strain energy such that: 1 r eE 2 ij ij ¼ 12rij eeij ð16Þ where eE ¼ ee þ eed is the total elastic strain recovered during unloading and ee is the eﬀective elastic strain. The total elastic strain energy is assumed to be a decomposition of two parts: the ordinary elastic strain Fig. 5. Fictitious uniaxial stress–strain elastic response where all the damage strain is recoverable. (a) All damage is recoverable (all cracks are closed but not healed), (b) eﬀective conﬁguration where all damage is removed. 2620 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 energy (1=2ree ) and the elastic-damage strain energy (1=2reE 1=2ree ). This signiﬁes that the stored elasticdamage energy is needed to open the closed cracks during the elastic loading. Substituting Eq. (12) into Eq. (16), the following relation between the eﬀective elastic strain, ee , and the total elastic strain, eE , is obtained as follows: eeij ¼ ð1 /ÞeEij ð17Þ This is analogous to the relation derived by Voyiadjis and Kattan (1992a). However, in that work the strain eE was not explicitly decomposed into its components ee and eed . A similar relation between the ordinary elastic strain, ee , and the eﬀective elastic strain, ee , can be obtained by substituting Eqs. (12) and (13) into Eq. (15) such that: eeij ¼ ð1 /Þeeij ð18Þ From the above relation it is clear that the eﬀective elastic strain, ee , is not identical to the ordinary elastic strain, ee , obtained through the additive strain decomposition in Eq. (7). This relation shows that the elastic strain (excluding the damage strain) depends on the damage level, which conforms well to the experimental observations that show the elastic strain decreases as the damage level increases, in particular, at strains close to failure, see Fig. 6. Furthermore, by rearranging Eq. (17) and substituting into Eq. (18) one obtains: eeij ¼ ð1 /Þ2 eEij ð19Þ which again emphasizes the previous result, see Fig. 6. Considering the additive decomposition of the total elastic strain, Eq. (7), into Eq. (19) and simplifying the result we obtain a relation for the elastic-damage strain, eed , as follows: " # 2 1 ð1 /Þ ed eij ¼ ð20Þ eeij 2 ð1 /Þ or by utilizing Eqs. (18) and (19) one obtains the following relation: " # 2 1 ð1 /Þ ed eij ¼ eeij ¼ ½1 ð1 /Þ2 eEij ð1 /Þ ð21Þ This relation shows that the elastic-damage strain, eed , increases with the damage growth (Fig. 6), which qualitatively agrees with the loading–unloading uniaxial tensile processes. Fig. 6. Variation of the diﬀerent types of elastic strain with respect to the damage variable, /. (a) With respect to the total elastic strain, (b) the elastic-damage strain to elastic strain ratio. R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2621 Finally, by substituting Eqs. (10) and (17) into Eq. (15) and comparing the result with Eq. (14), one derives a relation between the elastic-damage modulus, E, and the initial elastic modulus, E, in terms of the scalar damage variable, /, as follows: Eijkl ¼ Eijkl ð1 /Þ 2 ð22Þ This coincides with the relation obtained by Voyiadjis and Kattan (1992a). In Fig. 6(a) the variation of the strain ratios in the elastic range of Eqs. (17), (19) and (21) are plotted with respect to the damage variable, /. In Fig. 6(b) the variation of the strain ratio in the elastic range of Eq. (20) is plotted with respect to the damage variable, /. Fig. 6 shows a qualitatively correct behavior with respect to the experimental observations. It is noteworthy that if the damage variable, /, is known, one can then calculate the corresponding damage strain and stiﬀness using the derived equations. Next, we will demonstrate the proposed damage concept for the anisotropic case. 3.2. Anisotropic damage Many researchers tend to adopt the traditional simple isotropic scalar damage variable, ‘‘(1 /)’’, in order to model the material microdamage mechanism, in which all components of the material stiﬀness are degraded by the same scalar damage parameter, / (e.g. Krajcinovic and Foneska, 1981; Krajcinovic, 1983; Kachanov, 1986; Lemaitre and Chaboche, 1990; Lemaitre, 1992; Doghri, 2000; etc.). However, in order to insure a more realistic application of the principles of the damage mechanics, anisotropic damage should be assumed. In this case diﬀerent levels of damage are related to the principal directions, and thus a simple scalar damage parameter is no longer suﬃcient to quantify damage in all directions. Instead, the anisotropic phenomenon of the microdamage distribution in the material is interpreted using a symmetric second-order damage tensor, /ij (e.g. Murakami and Ohno, 1981; Murakami, 1983, 1988; Ortiz, 1985; Chow and Wang, 1987, 1988; Lubarda and Krajcinovic, 1993; Voyiadjis and Abu-Lebdeh, 1993; Voyiadjis and Kattan, 1992a,b; Voyiadjis and Venson, 1995; Voyiadjis and Park, 1997, 1999; Seweryn and Mroz, 1998; Voyiadjis and Deliktas, 2000; etc.). We now generalize the deﬁnition of the isotropic damage variable described above (Fig. 4) for the anisotropic case. Consider a damaged solid in which an RVE of ﬁnite volume has been isolated. Assume the RVE is an elementary parallelopiped, and consider facets of outward unit normal ni ði ¼ x; y; zÞ. Each of D the three facets has a diﬀerent evolution of microdamage; i.e. AD x on the facet that has a unit normal nx , Ay D on the facet that has a unit normal ny , and Az on the facet that has a unit normal nz . The total area of the facet in the nx , ny , and nz directions are designated as Ax , Ay , Az , respectively. A measure of damage in the RVE is then given by a second-order tensor deﬁned as follows: pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃ ð23Þ / ¼ q q or /ij ¼ qi qj where q is the microdamage (microcracks and microvoids) density, and deﬁned as follows: qi ¼ AD i Ai ðno sum on iÞ ð24Þ where AD i ði ¼ x; y; zÞ is the total area of the defects traces on the facet whose unit normal is ni . We will see in the subsequent sections that the deﬁnition of the strain energy release rate enables us to avoid calculation of AD i which would be extremely diﬃcult to do because of the lack of knowledge of the precise geometry of the microcracks and microvoids. A compound deﬁnition for damage was previously deﬁned by Kattan and Voyiadjis (2001) were both damages due to cracks and voids were superimposed. Their deﬁnition of voids followed the concept of area reduction due to damage. 2622 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 The damage tensor / in Eq. (23) can be written in a matrix form as follows: 2 3 2 pﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3 qx qx qy qx qz /xx /xy /xz ﬃﬃﬃﬃﬃﬃﬃﬃﬃ p pﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ qy qy qz 5 ½/ ¼ 4 /yx /yy /yz 5 ¼ 4 qy qx pﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃ qz qx qz qz qy /zx /zy /zz ð25Þ which is a generalization of the KachanovÕs parameter that has in some simple special cases the same meaning. In the work of Voyiadjis and Venson (1995) crack densities as a measure of microcracks only without microvoids was considered. In a later work by Voyiadjis and Kattan (1999), and Kattan and Voyiadjis (2001) the two types of damages were incorporated under the same variable, /. In the present work all the defect traces that evolve on the RVE facets (i.e. microcracks and microvoids) are considered. It is worth to say that the above deﬁnition is deﬁned from a pure geometric point of view; that is the larger the surface damage traces, the more severe the damage. From the material point of view, the distribution (spacing and orientation) and size of the surface damage traces have a considerable inﬂuence on the material behavior. For example the same total damaged area can be contributed by a smaller number of large voids/cracks or a larger number of small voids/cracks. Those eﬀects are implicitly considered in the evolution equations derived in the subsequent sections. This implicit consideration comes from the fact that the proposed model follows the phenomenological approach because the material behavior is described through a suitable set of internal variables, acting at the microstructural level, and whose relation to micromechanical processes is not exactly deﬁned. However, an explicit consideration of such eﬀects can be achieved by the use of the non-local or gradient damage theories (e.g. Pijaudier-Cabot and Bazant, 1987; Aifantis, 1992; Zbib and Aifantis, 1992; Voyiadjis et al., 2001; Taylor et al., 2002). This explicit consideration of the shape, size, and distribution of microcracks and microvoids by the use of the non-local or gradient theories can be easily adapted to the proposed model, but the matter is beyond the scopes and the limits of the present paper. One can write the linear elastic constitutive equations for the damaged material according to the principle of strain energy equivalence between the virgin material and damaged material (Sidoroﬀ, 1981). That is, the damaged material is modeled using the constitutive laws of the eﬀective undamaged material in which the Cauchy stress tensor, r, is replaced by the eﬀective stress tensor, r (Murakami and Ohno, 1981): rij ¼ Mikjl rkl ð26Þ where M is the fourth-order damage-eﬀect tensor. Many diﬀerent expressions for M have been proposed in the literature in order to symmetrize the eﬀective stress tensor, r. A comprehensive review of the most widely used expressions are presented by Voyiadjis and Park (1997). The following expression for M, which is proposed by Cordebois and Sidoroﬀ (1979), is used here due to its attractiveness in the mathematical formulations, such that: Mikjl ¼ 2½ðdik /ik Þdjl þ dik ðdjl /jl Þ1 ð27Þ where dij is the Kronecker delta. Furthermore, using the strain energy equivalence principle, Eq. (17) which relates the eﬀective elastic strain tensor ee with the total elastic strain tensor eE can be expressed for anisotropic damage as follows: 1 E eeij ¼ Mikjl ekl ð28Þ Also similar to Eq. (18), one can write: eeij ¼ Mikjl eekl ð29Þ Analogous to Eq. (22), the elastic-damage stiﬀness, E, can be rewritten using the fourth order damage-eﬀect tensor M as follows (Voyiadjis and Park, 1999): R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 1 1 Eijkl ¼ Mimjn Emnpq Mpkql 2623 ð30Þ where 1 Mikjl ¼ 12½ðdik /ik Þdjl þ dik ðdjl /jl Þ ð31Þ and E is the fourth-order elastic moduli tensor given by: Eijkl ¼ Kdij dkl þ 2Gðdik djl 13dij dkl Þ ð32Þ where K and G are the elastic bulk and shear moduli, respectively. Analogous to Eq. (21) one can express eed in terms of the applied stress, r, by substituting Eqs. (13) and (14) into Eq. (7), such that: 1 1 eed ij ¼ ðEijkl E ijkl Þrkl where E 1 and E 1 ð33Þ are the inverse counterparts of Eqs. (30) and (32), respectively. 3.3. The strain energy release rate ðGÞ The strain energy release rate G for the isotropic damage case is deﬁned as the rate of change in the elastic E potential energy density W with respect to the speciﬁc damaged area AD for a linear elastic material, such that: E G¼ oW oAD ð34Þ Now, we illustrate the derivation of the strain energy release rate G in one dimension. Consider an elasE tically loaded body containing microdamages (Fig. 5). The potential energy W for damage growth is given by: E W ¼U W ð35Þ where U is the strain energy stored in the body (reE =2) and W is the additional energy necessary for damage E growth and obtained from the work done by reE . The potential energy W , therefore, can be written as follows: E W ¼ 12reE ð36Þ Eq. (34) is obtained when the loading is stress controlled (the displacement is ﬁxed). However, if the loading E is strain controlled (the load is ﬁxed), the potential energy W is given as: E W ¼ 12reE Now substitution of Eq. (37) into Eq. (34) along with eE ¼ r=E, yields the following expression: 1 2r or 1 2 o G¼ þr D D 2 E oA oA E ð37Þ ð38Þ The stiﬀness of the body E is decreasing whether the body is rigidly gripped (strain control) such that the damage growth would result in a stress drop or whether the stress is ﬁxed (stress control) such that the damage growth would result in a strain increase. For the strain control case, both r and E would decrease, but the ratio r=E would remain the same, such that: 2624 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 1 or o þr D E oAD oA 1 ¼0 E ð39Þ using the above equation with Eq. (38), the following expression is obtained for G, such that: 1 o 1 G ¼ r2 D 2 oA E ð40Þ E In the case of stress control or strain control loading, the magnitude of W is equivalent as given by Eqs. (36) and (37). Thus, under ﬁxed stress loading condition the strain energy release rate is the same as given by Eq. (40), only the sign is reversed, reﬂecting the fact the G is independent of the type of load application (e.g. displacement control, load control, combinations of stress change and strain change). We found for the case of isotropic damage (Eq. (22)) that E for one-dimension can be expressed in terms of the undamaged stiﬀness E and the damage variable / as follows: E ¼ Eð1 /Þ 2 ð41Þ with / ¼ AD =A is given by Eq. (11). Substitution of Eq. (41) into Eq. (40), yields the following expression for the energy release rate G: G¼ r2 AEð1 /Þ 3 ð42Þ By substituting the nominal stress r from Eq. (10) along with the elastic strain energy equivalence principle (Eq. (16)), the strain energy release rate G can be written as a function of the energy potential and the damage variable as follows: E 2W G¼ Að1 /Þ ð43Þ The strain energy release rate for the anisotropic damage can be deﬁned as follows: E Gij ¼ oW oAD ij ð44Þ D D where AD ij ¼ Ai Aj as deﬁned in Eq. (23). Similar to the procedure outlined above, one can derive the strain energy release rate for the anisotropic damage case (G) with the aid of the deﬁnition presented by Eqs. (23), (30) and (31). Assuming that the total area of the RVEÕs facets in the nx , ny , and nz normals are constant, one can write G as follows: E Gij ¼ 2W Mkplq 1 oMkplq o/ab o/ab oAD ij ð45Þ Using Eq. (27), one can write: 1 oMkplq ¼ Jkplqab o/ab where J is a sixth-order tensor and is given by: Jkplqab ¼ 12 dlq dka dpb þ dkp dla dqb Hence, Eq. (45) can be written as: ð46Þ ð47Þ R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 E Gij ¼ 2W Mkplq Jkplqab o/ab oAD ij 2625 ð48Þ E where W is given by: E 1 1 W ¼ 12rij Eijkl rkl ¼ 12rij Eijkl rkl ð49Þ E It is noteworthy that since the magnitude of W is path independent as was shown in the beginning of this section, the expression of G does not diﬀer whether the imposed loading is strain control or stress control. This particularly agrees well with the deﬁnition of strain energy release rate made in fracture mechanics (Thomason, 1990; Anderson, 1994; Hertzberg, 1996). However, this does not imply that the strain energy release rate, presented in Eq. (43) for isotropic damage or Eq. (48) for anisotropic damage, is path independent. The expression for the strain energy release rate, which is used later to deﬁne the conjugate damage force, has in its composition the damage variable / which is path dependent. This makes both the strain energy release rate and the damage conjugate force path dependent. 4. Coupled damage/plasticity thermodynamic formulation 4.1. Helmholtz free energy density In this work, the elasto-plastic-damage material behavior is considered. This implies that stress path material dependence and the non-linear material response are considered. Thus, the dependent constitutive variables are functions of the total elastic strain tensor, eE , and nint - of internal state variables, @k ðk ¼ 1; . . . ; nint ; nint P 1Þ. Within the thermodynamic framework, the Helmholtz free energy density can be written as: W ¼ WðeEij ; @k Þ ð50Þ Since the main objective is to develop strong-coupled constitutive equations for a plastic-damaged material, the eﬀects of plastic strain hardening and microdamage mechanisms are to be considered. Experimental observations show that the accumulation of the material defects during the deformation process has a tendency to form macroscopically localized deformation regions. In those localized zones, many of defects may undergo irreversible growth; coalescence of pre-existing cracks and voids may occur; propagation of dislocations may proceed; and new defects may nucleate and their ultimate coalescence results in failure. Moreover, intensive interaction mechanisms of the evolved defects may take place at those localized zones; such as dislocation–dislocation interaction, microdamage–microdamage interaction, crack dominated–dislocation interaction, dislocation dominated–crack interaction, dislocation/crack–grain boundary interaction, etc. In order to consider such mechanisms in the constitutive equations, a ﬁnite set of internal state variables @k , acting at the microstructural level, representing either a scalar or a tensorial variable are assumed such that (Voyiadjis and Deliktas, 2000): @k ¼ @k ðaij ; p; Cij ; r; /ij Þ ð51Þ where a is the plastic ﬂux variable related to the kinematic hardening (movement of the loading surface), p is the equivalent plastic strain related to the isotropic hardening (size of the loading surface). Furthermore, since this work focuses on the development of a coupled plastic-damage framework based on the thermomechanical postulates, the various possibilities to describe anisotropic damage are to be presented here. The damage internal variables consist of the damage ﬂux variable C corresponding to the kinematic hardening (movement of the damage surface), r the cumulative inelastic-damage strain (size of the damage surface), and / the anisotropic damage tensor. p and r can be expressed as follows: 2626 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 Z t rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3 p p p¼ e_ e_ dt 2 ij ij 0 r¼ Z t qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ id e_id ij e_ij dt ð52Þ ð53Þ 0 Using the Clausius–Duhem inequality for isothermal state, one obtains: rij e_ij qw_ P 0 ð54Þ where q denotes the mass density. In Eq. (54) the total strain rate tensor, e_ , is decomposed into two parts: total elastic part, e_ E ¼ e_ e þ e_ ed and inelastic part, e_ I ¼ e_ p þ e_ id . The time derivative of Eq. (50) with the respect to its internal state variables, @k , is given by: _ ¼ oW e_E þ oW a_ ij þ oW p_ þ oW C_ ij þ oW r_ þ oW /_ ij W oeEij ij oaij op oCij or o/ij ð55Þ Substituting the rate of the Helmholtz free energy density, Eq. (55), into the Clausius–Duhem inequality, Eq. (54), along with Eq. (5), one obtains the following thermodynamic constraint: ! oW E oW oW oW _ oW oW _ / P0 rij q E e_ij þ rij e_Iij q Cij q ð56Þ p_ q r_ q a_ ij q oeij oaij op oCij or o/ij ij Eq. (56) results in the following thermodynamic state laws for the conjugate thermodynamic forces: rij ¼ q oW oeEij ð57Þ Xij ¼ q oW oaij ð58Þ R¼q oW op Hij ¼ q K¼q oW oCij oW or Yij ¼ q oW o/ij ð59Þ ð60Þ ð61Þ ð62Þ where X, R, H, K, and Y are the thermodynamic forces conjugate to the ﬂuxes a, p, C, r, and /, respectively. The complexity of a model is directly determined by the form of the Helmholtz free energy W and by the number of conjugate pairs of variables. The speciﬁc free energy, W, on the long-term manifold (neglecting the short-term manifolds) is assumed as follows: 1 1 1 1 1 qW ¼ eEij Eijkl ð/ÞeEkl þ Caij aij þ Q p þ ebp þ aCij Cij þ q r þ ecr ð63Þ 2 3 b 2 c R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2627 where Eð/Þ is the fourth-order damage elastic tensor and C, Q, b, a, and c are material-dependent constants. The form of the ﬁrst term in Eq. (63) has been often postulated in damage mechanics, and is based on the concept of the eﬀective stress r so that it presents the same strain or the same elastic energy as a damaged element subjected to the nominal stress r. The rest of the terms in Eq. (63) have been assumed in this form in order to derive non-linear evolution equations for the isotropic and kinematic hardening that describe more accurately the plasticity and damage deformation mechanisms. Where the second and third terms take a form as proposed by Chaboche (1989). The forth and ﬁfth terms are assumed analogous to the second and third terms, respectively for the case of damage. The proposed deﬁnition of W allows the derivation of the constitutive equations and the internal dissipation described next. The state laws of the assumed internal state variables are obtained by substituting Eq. (63) into Eqs. (57)–(61), such that: rij ¼ Eijkl ðekl epkl eid kl Þ ð64Þ Xij ¼ 23Caij ð65Þ R ¼ Qð1 ebp Þ ð66Þ Hij ¼ aCij ð67Þ K ¼ qð1 ecr Þ ð68Þ Now, one can obtain an expression for the damage driving force Y in terms of the strain energy release rate presented in Eq. (45). By using the chain rule, the thermodynamic state law of Y (Eq. (62)) can be written as follows: Yij ¼ q oWE oAD mn oAD mn o/ij ð69Þ Using the deﬁnition of strain energy release rate for anisotropic damage (Eq. (44)) and the physical deﬁnition of the damage tensor / (Eqs. (23) and (24)) along with the assumption of A designating the total area of the RVEÕs facets in the nx , ny , and nz directions, one can write Eq. (69) in terms of the strain release rate, G, as follows: Yij ¼ Gmn oAD mn o/ij ð70Þ Substituting the expression derived for the strain energy release rate for anisotropic damage G (Eq. (48)) into Eq. (70), one can express the damage driving force Y as follows: E Yij ¼ 2W Mkplq Jkplqij E ð71Þ E where W and J are given by Eqs. (47) and (49), respectively. we may replace W ¼ r : ee =2 by pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃFurthermore, ﬃ its expression in terms of equivalent stress req ¼ 3s : s=2 and the hydrostatic stress P ¼ tracðrÞ=3 as follows: r2eq 2 9P W ¼ þ 6G 2K E ð72Þ where K ¼ 3E=ð1 2mÞ, G ¼ E=2ð1 þ mÞ, and m is the PoissonÕs ratio. For the isotropic damage case we may write an expression for Y as follows: 2628 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2 Y ¼ 2 r r ¼ Eð1 /Þ Eð1 /Þ ð73Þ with 2 1=2 r ¼ req ½23ð1 þ mÞ þ 3ð1 2mÞðP =req Þ ð74Þ where r ¼ ð1 /Þr . This is referred to as the equivalent damage stress according to the notation by Lemaitre and Chaboche (1990). The ratio P =req expresses the triaxiality of the state of stress. 4.2. The dissipation function and the maximum dissipation principle Using the equations of state (Eqs. (57)–(62)), the Clausius–Duhem inequality expression (Eq. (56)) becomes: _ ij Rp_ Hij C_ ij K r_ þ Yij /_ ij P 0 P ¼ rij ðe_pij þ e_id ij Þ Xij a ð75Þ where P deﬁnes the dissipation due to plasticity and damage morphologies and requires to be non-negative. It can be seen from the dissipation function P that both irreversible and reversible damage strains cause energy dissipation. The irreversible strains through r : e_ id and the reversible strains through Y : /_ . The rate of the internal state variables associated with plastic and damage deformations are obtained by utilizing the calculus of functions of several variables with the Lagrange multipliers k_p and k_d , respectively. The dissipation function P (Eq. (75)) is subjected to the two constraints, namely f ¼ 0 and g ¼ 0 (Voyiadjis and Kattan, 1992a), such that: X ¼ P k_p f k_d g ð76Þ One now can make use of the maximum dissipation principle (Simo and Honein, 1990; Simo and Hughes, 1998), which states that the actual state of the thermodynamic forces (r, Y ) is that which maximizes the dissipation function over all other possible admissible states. Thus, we maximize the objective function X by using the necessary conditions as follows: oX ¼0 orij and oX ¼0 oYij ð77Þ Substitution of Eq. (76) into Eq. (77) along with Eq. (75) yields the thermodynamic laws corresponding to the evolution of the total inelastic strain rate (eI ) and the damage variable (/), where Eq. (77)1 gives the inelastic strain rate as follows: of og e_Iij ¼ k_p þ k_d orij orij ð78Þ Considering the earlier postulate of the additive decomposition of the inelastic strain rate into plastic and damage parts, Eq. (8), the following assumption is made: e_pij ¼ k_p of orij and _d e_id ij ¼ k og orij ð79Þ This assumption suggests that the inelastic-damage strains, eid , may be anticipated even before any plastic deformation can be observed, which qualitatively meets the discussion outlined in Section 2. On the other hand, Eq. (77)2 gives the damage rate evolution law as follows: of og /_ ij ¼ k_p þ k_d oYij oYij ð80Þ R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2629 Eq. (80) signiﬁes, once again, that the damage growth occurs even if there is no plastic ﬂow (i.e. k_p ¼ 0), which agrees well with the experimental observations in brittle materials and justiﬁed in Fig. 5. In order to obtain non-associative rules for the damage and plasticity hardening variables, one can assume the existence of a plastic potential F and a damage potential G such that they are respectively not equal to f and g. This postulate is essential in order to obtain non-linear plastic and damage hardening rules, which give a more realistic characterization of the material response in the deformation process. The complementary laws for the evolution of the other internal state variables can then be obtained directly from the generalized normality rule, such that: oF a_ ij ¼ k_p oXij ð81Þ oF p_ ¼ k_p oR ð82Þ oG C_ ij ¼ k_d oHij ð83Þ oG r_ ¼ k_d oK ð84Þ where k_p and k_d are determined using the consistency conditions f_ ¼ 0 and g_ ¼ 0, respectively. The next step is the selection of the appropriate form of the plastic potential function F , the plastic yield surface f , the damage potential function G, and the damage growth surface g in order to establish the desired constitutive equations that describe the mechanical behavior of the material. 4.3. Plasticity and damage dissipation potentials and hardening rules 4.3.1. Plastic dissipation potential and hardening rules Once a material is damaged, further loading can only aﬀect the undamaged material. Thus, the damage potential function G is deﬁned in terms of the eﬀective stresses and strains. By combining plasticity with damage, it seems natural that plasticity can only aﬀect the undamaged material skeleton. Thus plastic potential F is also deﬁned in terms of the eﬀective stresses and strains. The plastic potential F is deﬁned as: F ¼f þ 3 c X ij X ij 4C ð85Þ where c and C are material constants used to adjust the units of the equation. f is of a von Mises type given as follows: rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3 ðsij X ij Þðsij X ij Þ ryp RðpÞ ¼ 0 f ¼ ð86Þ 2 where ryp is the initial size of the yield surface, and s and X are expressed in terms of the damage tensor M (given by Eq. (27)) and the corresponding damage states as follows (Voyiadjis and Kattan, 1999): 0 sij ¼ Mikjl rkl 0 where Mikjl ¼ Mikjl 13Mrkrl dij ð87Þ and X ij ¼ Mikjl Xkl ð88Þ 2630 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 The plastic parameter k_p P 0, which is known as the plastic consistency parameter, is assumed to obey the following Kuhn–Tucker loading/unloading conditions: 8 9 8 < < 0 ) k_p ¼ 0 = < elastic unloading ð89Þ f 6 0 and f_ ¼ 0 ) k_p ¼ 0 () neutral loading : ; : p _ plastic loading ¼0)k >0 In order to derive the evolution of the plasticity isotropic hardening function, the time rate of Eq. (66) gives: R_ ¼ bQp_ ebp A relation between R and p can be obtained from Eq. (66), such that: 1 R p ¼ ln 1 b Q ð90Þ ð91Þ which upon substituting it into Eq. (90) yields the following expression for R_ , such that: R_ ¼ b½Q Rp_ ð92Þ The isotropic hardening represents a global expansion in the size of the yield surface with no change in shape. Thus for a given yield criterion and ﬂow rule, isotropic hardening in any process can be predicted from the knowledge of the function R, and this function may in principle, be determined from a single test (e.g. the tension test). Therefore, the eﬀective isotropic hardening function R is related to the nominal isotropic hardening function by Eq. (10) as follows: R¼ R 1 /eq where (Voyiadjis and Park, 1997) qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ /eq ¼ /ij /ij ð93Þ ð94Þ Using Eq. (82) along with the chain rule and Eqs. (86) and (93), it can be easily shown that p_ is related to k_p by: k_p ¼ ð1 /eq Þp_ ð95Þ Using the chain rule and Eq. (88), Eq. (81) is now expressed as follows: oF a_ ij ¼ k_p Mminj oX mn Substitution of Eq. (85) into the above equation yields: of 3 c X mn þ a_ ij ¼ k_p Mminj oX mn 2 C ð96Þ ð97Þ since of =oX ¼ of =or as it is clear from Eq. (86), it is easily shown with using the chain rule and Eqs. (26), (79)1 , (88) together with the time rate of Eq. (65) that the evolution equation of the plastic kinematic hardening X_ is related to e_ p , X, and M as follows: X_ ij ¼ 23C e_pij ck_p Mminj Mmrns Xrs ð98Þ Substituting Eq. (95) into the above equation, gives the following form for the evolution equation of the backstress tensor X_ , such that: R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 X_ ij ¼ 23C e_pij cð1 /eq ÞMminj Mmrns Xrs p_ 2631 ð99Þ 4.3.2. Damage dissipation potential and hardening rules The anisotropic damage governing equations are formulated in spirit of plasticity. Thus, analogous to the plasticity potential function F , one can assume the following form of the damage potential function G in the space of the damage forces and the conjugated forces of the hardening variables (Voyiadjis and Deliktas, 2000): G¼gþ 1d Hij Hij 2a ð100Þ where d and a are material constants used to adjust the units of the equation. g is the damage growth function postulated as follows: qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ g ¼ ðYij Hij ÞðYij Hij Þ ld KðrÞ ¼ 0 ð101Þ where ld is the initial damage threshold. The damage consistency parameter k_d P 0 is assumed to obey the following Kuhn–Tucker conditions: 8 9 8 < < 0 ) k_d ¼ 0 = < undamaged state ð102Þ g 6 0 and g_ ¼ 0 ) k_d ¼ 0 () damage initiation : ; : damage growth ¼ 0 ) k_d > 0 Using Eq. (84) along with Eq. (101), the following relation is obtained: k_d ¼ r_ ð103Þ Taking the time rate of Eq. (68) and expressing r in terms of K, the evolution of the damage isotropic hardening function K can be easily written as: K_ ¼ cðq KÞ_r ð104Þ Now, one can derive an expression for the damage kinematic hardening rule by taking the time rate of Eq. (67) and making use of Eqs. (80), (83), (100) and (103) such that: og H_ ij ¼ a dHij r_ ð105Þ oYij Next, explicit expressions for the plasticity and damage Lagrange parameters k_p and k_d are derived using the consistency conditions f_ and g_ , respectively. 4.4. Plasticity and damage consistency conditions Since r, X, and R are functions of / and their corresponding nominal counter parts r, X, and R, it follows that the yield function f may be expressed as a function /, such that the corresponding consistency condition f_ ¼ 0 can be written as follows: of of _ of _ of _ Rþ / ¼0 Xij þ f_ r_ ij þ orij oXij oR o/ij ij ð106Þ By assuming that the elastic-damage stiﬀness, E, is constant within each stress/strain increment, which is the case in the strain-driven problem, one can write the time rate of the Cauchy stress tensor (r_ ) as follows: r_ ij ¼ Eijkl e_Ekl ð107Þ 2632 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 Making use of the above equation, Eqs. (78), (80), (86), (92), (93), (95), (99), and the chain rule with noticing that of =oX ¼ of =or, it can be shown, after some manipulation, that the consistency condition, Eq. (106), gives the following relation between k_p and k_d , such that: a11 k_p þ a12 k_d ¼ b1 ð108Þ where a11 ¼ of of 2 of of of of of bðQ RÞ Eijkl þ C c Mminj Mmrns Xrs þ orij orkl 3 orij orij orij o/ij oYij ð1 /eq Þ2 ð109Þ a12 ¼ of og of og Eijkl orij orkl o/ij oYij ð110Þ and b1 ¼ of Eijkl e_kl orij ð111Þ On the other hand, the consistency condition for the damage, g_ ¼ 0, can be written as follows: g_ og _ og _ og _ K¼0 Yij þ Hij þ oYij oHij oK ð112Þ However, since the damage driving force Y is a function of r and / (see Eq. (71)), the damage consistency condition can be rewritten as follows: g_ og og _ og _ og _ Kþ / ¼0 Hij þ r_ ij þ orij oHij oK o/ij ij ð113Þ Making use of Eqs. (78), (80), (101) and (103)–(105) along with the chain rule, it can be shown, after some manipulation, that the consistency condition, Eq. (113), gives the following relation between k_p and k_d , such that: a21 k_p þ a22 k_d ¼ b2 ð114Þ where a21 ¼ og of og of Eijkl orij orkl o/ij oYij ð115Þ a22 ¼ og og og og og Eijkl d Hij þ cðq KÞ þ a orij orkl oYij o/ij oYij ð116Þ and b2 ¼ og Eijkl e_kl orij ð117Þ The plastic multiplier, k_p , and the damage multiplier, k_d , can be found from the linear system of equations given by Eqs. (108) and (114) such that: p 1 a22 a12 b1 k_ ¼ ð118Þ b2 D a21 a11 k_d R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2633 where D ¼ a11 a22 a12 a21 ð119Þ 4.5. The elasto-plastic-damage tangent stiﬀness Substituting k_p and k_d from Eq. (118) into Eq. (78), the evolution equation for the inelastic strain rate e_ I can be written in the following form: e_Iij ¼ vijkl e_kl ð120Þ where v is a fourth-order tensor and is expressed as follows: vijkl ¼ Pijkl þ Zijkl ð121Þ where Pijkl ¼ of Ars Erskl orij ð122Þ Zijkl ¼ og Brs Erskl orij ð123Þ 1 of og a22 a12 D orrs orrs ð124Þ 1 og of a11 Brs ¼ a21 D orrs orrs ð125Þ Ars ¼ Substitution of Eqs. (120) and (33) into Eq. (107), yields the following: r_ ij ¼ Dijkl e_kl ð126Þ where D represents the elasto-plastic-damage tangent stiﬀness given by: Dijkl ¼ Eijkl Eijmn vmnkl The tangent stiﬀness D has two possible expressions, such that: ( Eijkl ; if f < 0 or f_ < 0 and g < 0 or g_ < 0 Dijkl ¼ Eijkl Eijmn vmnkl if f ¼ 0 () k_p f_ ¼ 0 or g ¼ 0 () k_d g_ ¼ 0 ð127Þ ð128Þ The above expression signiﬁes that D ¼ E if there is no damage and no plastic ﬂow; and D ¼ E if there is total crack closure, total void contraction, and no plastic ﬂow. For the sake of completeness we outline in Appendix A the derivatives that are necessary to calculate the above evolution equations. 5. Qualitative and quantitative results The pure damage and the coupled plastic-damage model behavior are examined in the sequel for the case of isotropic damage. The new features that the proposed model is attempting to represent are illustrated by providing qualitative and quantitative plots of stress versus strain. 2634 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 5.1. The case of pure isotropic damage In this section some properties of the damage model proposed in Section 4.3.2 are investigated for some simple uniaxial processes using a dissipation mechanism produced by the damage potential only. The damage criterion with linear isotropic damage hardening is considered such that Eq. (101) can be expressed as follows: g¼ Eð1 /Þ3 ð1 þ /Þ 2 e2 ld q/ ¼ 0 ð129Þ where e ¼ ee þ eed þ eid is the total strain, ld is the damage threshold, and q is the damage hardening modulus. The evolution of the damage variable / in uniaxial extension can be obtained from Eq. (129) for a given e, ld , and q. The limit uniaxial strain and stress at which damage initiates are obtained by setting / ¼ 0 in Eq. (129) such that: qﬃﬃﬃﬃﬃﬃﬃ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð130Þ e0 ¼ ld =E; r0 ¼ Eld The elastic strain, ee , the elastic-damage strain, eed , and the inelastic-damage strain, eid , can be obtained from the relations presented in Section 3.1 and Eq. (79)2 such that: ee ¼ ð1 /Þ3 e; ð1 þ /Þ eed ¼ ð1 /Þ ð1 /Þ3 e; ð1 þ /Þ eid ¼ 2/ e 1þ/ ð131Þ For / ¼ 0, ee ¼ e and eed ¼ eid ¼ 0. The stress relation follows from the elastic constitutive relation: 3 r ¼ Dsec e with Dsec ¼ ð1 /Þ E ð1 þ /Þ ð132Þ The stress–strain curves are shown in Fig. 7 for diﬀerent values of the damage threshold ld and the damage hardening modulus q. It is evident that the model allows simulating a continuous change from hardening to softening as well as the reduction in the stiﬀness. It is noteworthy that the energy necessary to initiate the damaged state (that can be interpreted as fracture energy Gf ) is ﬁnite, in fact: Z e0 1 1 r de ¼ Ee20 ¼ ld ð133Þ Gf ¼ 2 2 0 Therefore, for q ¼ 0, Eq. (129) characterizes a fracture-type criterion. Moreover, it can be noted from Fig. 7(b) that for q ¼ 0 (i.e. no damage hardening), for each / there is a unique value of stress; while for q 6¼ 0 (i.e. with damage hardening), for each / there are two possible stress values. Therefore, due to the Fig. 7. Inﬂuence of the (a) ld parameter and (b) q (Mpa) parameter for E ¼ 199 GPa. R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2635 presence of damage the application of this model to structural problems will cause strain localization with the consequent mesh-dependency of the numerical results. Several regularization approaches, either in time or space, have been proposed in the literature to accommodate this problem (see Voyiadjis et al., 2001). However, the purpose of this study is to introduce the model and the possible strategies for coping with strain localization are beyond the goal of the present work. The loading–unloading behavior is considered in Fig. 8(a). When damage occurs, it can be seen upon unloading that there is a permanent strain in the stress free state. This qualitatively agrees with the experimental observations in concrete (Van Mier, 1984), where plasticity is assumed to be negligible. The stress–strain plot in Fig. 8(a) with damage hardening is obtained for very large value of q ¼ 50 MPa so that the secant stiﬀness, Dsec , after ﬁrst damage does not degrade immediately, as it has been observed in some experimental tests on concrete. Hardening then decreases fast as soon as damage localization develops. Fig. 8(b) shows the variation of the diﬀerent coupled-damage strains with respect to the damage variable /. Fig. 8 shows an important feature of the proposed damage model that has not been considered by most of the previous models. Furthermore, it can be seen that for the same corresponding imposed strain, the elastic-damage modulus is bigger for pure damage with hardening than without hardening. This implies an increase in the material strength due to interaction between microdamages. This is also a new aspect was not provided by many of the previous damage models. The inﬂuence of the hardening modulus q is shown in Fig. 9 for ld ¼ 3:0 MPa and E ¼ 199 GPa. The evolution of / and the elastic-damaged modulus E are also reported. Increasing values of q determine stronger reduction in / and stronger increase in E. The parameter q particularly inﬂuence the degradation Fig. 8. Damage hardening eﬀect. (a) Loading–unloading uniaxial tensile process, (b) variation of diﬀerent type of strains with damage, for E ¼ 199 GPa and ld ¼ 3 MPa. Fig. 9. (a), (b) Inﬂuence of q (MPa) parameter for E ¼ 199 GPa and ld ¼ 3 MPa. 2636 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 of the elastic modulus and the concavity of the stress–strain curve Eð/Þ that can be obtained from experiments (Fig. 9). 5.2. Coupled plasticity and damage––application to high strength steel In this section the experimental results of Hesebeck (2001) for a high strength steel are numerically simulated using the proposed model. The tested high strength steel 30CrNiMo8 contains 33% carbon. Further details of the chemical composition are documented in Hesebeck (2001). In the mechanical experiments, force controlled tension tests with partial unloadings were performed at a stress rate r_ ¼ 30 MPa/s1 . The resulting stress versus strain curve obtained by Hesebeck (2001) is plotted in Fig. 10. Considering the fact that there are no uniﬁed experimental methods developed to quantify the damage variable, one can obtain / with suﬃcient precision by evaluating the unloading (i.e. the decrease in the stiﬀness) in the stress–strain curve, such that one can write from Eq. (22) the following expression: rﬃﬃﬃﬃ E /¼1 ð134Þ E Voyiadjis and Venson (1995) advocated the use of the sectioned specimens together with the use of the SEM for the determination of crack densities. However, diﬀerent interpretation of the experimental damage variable have been made by Hesebeck (2001), which is based on the strain equivalence principle (i.e. E ¼ Eð1 /Þ). However, the strain energy equivalence is considered in the present work. The result for the damage variable using Eq. (134) is plotted in Fig. 11 versus the elastic-damage modulus, E. Identiﬁcation of the material constants associated with any proposed material model is one of the most challenging issues for researchers in order to obtain better representation of their material models. The identiﬁcation approach of the material constants for the evolution equations outlined in the previous sections is based on the experimental results in Figs. 10–12 by using the least-squares minimization method. YoungÕs modulus, PoissonÕs ratio, and the initial ﬂow stress were pre-determined by Hesebeck (2001) as E ¼ 199 GPa, m ¼ 0:3, and ryp ¼ 870 MPa, respectively. The object of the identiﬁcation process here is to Fig. 10. Stress-strain diagram for damaged and eﬀective undamaged 30CrNiMo8-steel as compared to the experimental data. R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2637 Fig. 11. Elastic-damage modulus (E) versus damage variable (/). Fig. 12. Comparison of experiments by Hesebeck (2001) with the simulated data of the present work for the damage variable versus the inelastic strain. identify the four parameters (Q, b, C, c) of Eqs. (92) and (99), characterizing the plastic isotropic and kinematic hardening, and the ﬁve parameters (ld , q, c, d, a) of Eqs. (101), (104) and (105), characterizing the initial damage threshold, and damage isotropic and kinematic hardening. The plasticity hardening parameters are determined using the eﬀective stress-eﬀective plastic strain curve in Fig. 10, while the damage 2638 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 Table 1 The plasticity and damage material parameters for 30CrNiMo8 high strength steel Mechanism Isotropic hardening Kinematic hardening Initial ﬂow threshold Plasticity Damage Q ¼ 409 MPa b ¼ 9.3 q ¼ 8.2 MPa c ¼ 5.2 C ¼ 15,000 MPa c ¼ 37 a ¼ 14.70 MPa d ¼ 0.11 ryp ¼ 870 MPa ld ¼ 3.8 MPa parameters are determined using all the experimental data in Figs. 10–12. The obtained material parameters are listed in Table 1. Preliminary results not reported here revealed that the eﬀective stress-eﬀective plastic strain curve could be obtained with reasonable agreement with the experimental data by considering only the isotropic hardening evolution, but by using diﬀerent material parameters than those listed in Table 1. Nevertheless this is not a problem for the practical applicability of the developed model. The emphasis of this work is to understand better the diﬀerent deformation morphologies that aﬀect the material behavior by considering their synergetic eﬀects. Therefore, the inﬂuence of the diﬀerent cooperative phenomena on plasticity and damage growth are discussed here. The curves plotted in Figs. 13–15 represent the synergetic eﬀects of the combined isotropic and kinematic hardening associated with plasticity, combined isotropic and kinematic hardening associated with damage, and damage mechanisms. Fig. 10 depicts the resulting eﬀective stress versus the eﬀective plastic strain curve of the proposed model, thus revealing a very good agreement with the experimental data. Also, the true stress (r ¼ ð1 /Þr) versus the inelastic strain (eI ¼ ep =ð1 /Þ) curve is shown in Fig. 10. The results of the present work for the damage variable (/) versus the inelastic strain (eI ) are shown in Fig. 12 while considering the experimental calculation of the damage variable and using both the strain equivalence and the strain energy equivalence principles. Also for this type of data it becomes apparent that the proposed model is able to give a good agreement with the experimental data for the material under consideration. High non-linear dependency between / and eI is noticed in Fig. 10, which agrees well with the experimental observations. Fig. 13. Evolution of the plasticity dissipative forces using the present model. R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2639 Fig. 14. Evolution of the damage dissipative forces using the present model. Fig. 15. Variation of the strain decomposition with the damage variable. (a) Elastic strain decomposition, (b) inelastic strain decomposition. The evolution of the plasticity dissipative forces R and X , and the damage dissipative forces K, H , and Y are shown in Figs. 13 and 14, respectively. Closed form expressions have been derived for the plasticity and damage hardening forces by integrating Eqs. (92), (99), (104) and (105) over the uniaxial tensile stress– strain data. The damage force Y is simpliﬁed for the one-dimensional case by using Eq. (71). The calculated additive decomposition of the total elastic strain (eE ) into the ordinary elastic strain (ee ) and the elastic-damage strain (eed ) as a function of / is shown in Fig. 15(a). In addition, the calculated additive decomposition of the total inelastic strain (eI ) into the plastic strain (ep ) and the inelastic-damage strain (eid ) as a function of / is shown in Fig. 15(b). Fig. 15 shows qualitatively correct behavior as anticipated in the discussion outlined in Section 2. Although this study is restricted to small strains, usually up to 2–4%, the results in Figs. 10–15 are extended to inelastic strains up to 6%. However, the proposed model is in reasonable quantitative agreement with the experimental data for uniaxial loading and exhibits a qualitatively correct behavior for the 2640 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 evolution of the diﬀerent strain types. Moreover, one will ﬁnd in the literature considerable fewer published experimental results for multi-axial loadings. In this work uniaxial tension experimental data with unloadings are used to obtain the constitutive parameters of the proposed model. The reduction in the elastic stiﬀness, particularly, has been measured from the uniaxial case. Therefore, the present model, for the time being, cannot be tested for more general paths. This will presented in a forthcoming paper. 6. Conclusions In the current paper the systematic construction of a thermodynamic consistent model for ductile materials, which provides a strong coupling between plasticity and damage, is presented. The model considers the diﬀerent interaction mechanisms exhibited by the plasticity and the damage morphologies. Plasticity and damage combined isotropic and kinematic hardening are considered. In addition, an additive decomposition of the total strain into elastic, plastic, and damage parts is proposed in this work. The damage component is further decomposed into two parts, one is due to the crack closure and void contraction and the other is due to the lack of crack closure and void contraction. The later may be attributed to the geometrical constraints set up by the interacting microcracks, microvoids, dislocation densities, and grain boundaries. Although microstructural arguments are used to motivate many aspects of the formulation, the fact remains that the formulation is phenomenological. The material behavior is described through a suitable set of internal variables and whose relation to micromechanical structure and processes is not exactly deﬁned. A strong coupling between the two dissipative processes, plasticity and damage, is implemented. This strong coupling have been assessed by using two separate plasticity and damage surfaces with separate nonassociated ﬂow rules in such a way that both damage and inelastic ﬂow rules are dependent on the plastic and damage potentials. Two damage mechanisms have been considered, one mechanism is coupled with plasticity, and while the other one occurs independent of plastic deformation. The dissipation function of the latter occurs in both the elastic and plastic domains. Some of the new features of the proposed damage model that are not reﬂected in the current models are investigated for some simple uniaxial tensile processes. Moreover, uniaxial tension tests by Hesebeck (2001) with unloadings for a high strength steel have been used to investigate the coupled plastic-damage behavior. The proposed model is in a very good quantitative agreement with the experimental data for uniaxial loading and exhibits a qualitatively correct behavior for the evolution of the diﬀerent strain types. However, even though the veriﬁcation is based on limited set of data, namely that of uniaxial stress and strain, this could speciﬁcally motivate experimentalists to look for the new features that would provide justiﬁcation for the approach used in the current study. The eﬀects of crack closure and void contraction are considered in this work upon unloading. However, those eﬀects under compressive loading are not considered in this work, which will be the focus of a forthcoming paper. In addition, explicit treatment of the microdamage distribution (spacing and orientation) and size, which have a considerable inﬂuence on the interaction between defects, will be addressed in a future work by the authors. Future work should be directed for implementation of the proposed model in a ﬁnite deformation framework to model problems that exhibit non-homogenous deformation. In addition it will also be used to investigate the necessity of the proposed additive decomposition of the total strain into elastic, plastic, and damage parts. These additional investigations should be based on the results of micromechanical characterization of the materials that exhibit heterogenous behavior and on the experimental evidence obtained in the laboratory accompained by metallographic studies and stereology based quantiﬁcation methods using tomography images. Additional aspects for future work is the consideration of the diﬀerent behavior in tension and compression for damage. Moreover, the problem of size eﬀect, strain localization, and mesh R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2641 dependency, typical of damage evolution, has not been addressed in this paper. Some of these aspects are presented in Voyiadjis et al. (2003), Voyiadjis and Abu Al-Rub (accepted for publication) in the framework of the proposed formulation and the non-local damage theories. Appendix A The following relations are necessary for the model implementation: /ij of of ormn of oXmn of oR of þ þ ¼ Mmrns Jmpnqij Mpkql ðrkl Xkl Þ þ R 2 o/ij ormn o/ij oXmn o/ij oR o/ij orrs ð1 /eq Þ og og oYmn og oHmn og oK og þ þ ¼ o/ij oYmn o/ij oHmn o/ij oK o/ij oYmn oHmn W Mkalb Mrpsq Jarbsij Jkplqmn o/ij E ! a2 ðA:1Þ /ij /eq ðA:2Þ of of ormn of ¼ ¼ Mminj orij ormn orij ormn ðA:3Þ og og oYmn og ¼ eEij Mkplq Jkplqmn orij oYmn orij oYmn ðA:4Þ of of ormn of ¼ oYij ormn oYij ormn oYij ormn 1 ðA:5Þ where oYij ¼ Mkplq Jkplqij eEmn ormn ðA:6Þ og Yij Hij pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ oYij ðYkl Hkl ÞðYkl Hkl Þ ðA:7Þ of 3 sij X ij qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ orij 2 3 ðs X Þðs X Þ kl kl kl kl 2 ðA:8Þ References Aifantis, E.C., 1992. On the role of gradients in the localization of deformation and fracture. International Journal of Engineering Science 30, 1279–1299. Anderson, T.L., 1994. Fracture Mechanics: Fundamentals and Applications, second ed. CRC Press, USA. Chow, C.L., Wang, J., 1987. An anisotropic theory of continuum damage mechanics for ductile fracture. Engineering Fracture Mechanics 27 (5), 547–558. Chow, C.L., Wang, J., 1988. A ﬁnite element analysis of continuum damage mechanics for ductile fracture. International Journal of Fracture 38, 83–102. Chaboche, J.-L., 1989. Constitutive equations for cyclic plasticity and cyclic viscoplasticity. International Journal of Plasticity 5, 247– 302. Cordebois, J.P., Sidoroﬀ, F., 1979. Anisotropic damage in elasticity and plasticity. Journal de Mecanique Theorique et Appliquee, Numero Special, 45–60. 2642 R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 Doghri, I., 2000. Mechanics of Deformable Solids: Linear and Nonlinear, Analytical and Computational Aspects. Springer, Germany. Ehlers, W., 1995. A single-surface yield function for geomaterials. Archive of Applied Mechanics 65, 246–259. Gurson, A.L., 1977. Continuum theory of ductile rupture by void nucleation and growth. Part I: Yield criteria and ﬂow rules for porous ductile media. Journal of Engineering Materials and Technology 99, 2–15. Hansen, N.R., Schreyer, H.L., 1994. Thermodynamically consistent framework for theories of elastoplasticity coupled with damage. International Journal of Solids and Structures 31 (3), 359–389. Haj-Ali, R., Pecknold, D.A., Ghaboussi, J., Voyiadjis, G.Z., 2001. Simulated micromechanical models using artiﬁcial neural networks. Journal of Engineering Mechanics, ASCE 127 (7), 730–738. Hertzberg, R.W., 1996. Deformation and Fracture Mechanics of Engineering Materials, fourth ed. John Wiley & Sons. Hesebeck, O., 2001. On an isotropic damage mechanics model for ductile materials. International Journal of Damage Mechanics 10, 325–346. Kachanov, L.M., 1958. On the creep fracture time. Izv Akad, Nauk USSR Otd. Tech 8, 26–31 (in Russian). Kachanov, L.M., 1986. Introduction to Continuum Damage Mechanics. Martinus Nijhoﬀ Publishers, The Netherlands. Kattan, P.I., Voyiadjis, G.Z., 2001. Decomposition of damage tensor in continuum damage mechanics. Journal of Engineering Mechanics, ASCE 127 (9), 940–944. Krajcinovic, D., Foneska, G.U., 1981. The continuum damage theory of brittle materials. Journal of Applied Mechanics 48, 809–824. Krajcinovic, D., 1983. Constitutive equations for damaging materials. Journal of Applied Mechanics 50, 355–360. Krajcinovic, D., 1996. Damage Mechanics. Elsevier, Amsterdam. Lemaitre, J., 1984. How to use damage mechanics. Nuclear Engineering and Design 80, 233–245. Lemaitre, J., 1985. A continuous damage mechanics model for ductile fracture. Journal of Engineering Materials and Technology 107, 83–89. Lemaitre, J., Chaboche, J.-L., 1990. Mechanics of Solid Materials. Cambridge University Press, London. Lemaitre, J., 1992. A Short Course in Damage Mechanics. Springer-Verlag, New York. Li, Q.M., 2000. Energy correlations between a damaged macroscopic continuum and its sub-scale. International Journal of Solids and Structures 37, 4539–4556. Lubarda, V.A., Krajcinovic, D., 1993. Damage tensors and the crack density distribution. International Journal of Solids and Structures 30, 2859–2877. Lubarda, V.A., Krajcinovic, D., 1995. Some fundamental issues in rate theory of damage-elastoplasticity. International Journal of Plasticity 11, 763–797. Lubliner, J., 1990. Plasticity Theory. Macmillan Publishing Company, New York. Mahnken, R., 2002. Theoretical, numerical and identiﬁcation aspects of a new model class for ductile damage. International Journal of Plasticity 18, 801–831. Murakami, S., Ohno, N., 1981. A continuum theory of creep and creep damage. In: Proceedings of the Third IUTAM Symposium on Creep in Structures. Springer, Berlin, pp. 422–444. Murakami, S., 1983. Notion of continuum damage mechanics and its application to anisotropic creep damage theory. Journal of Engineering Mechanics and Technology 105, 99–105. Murakami, S., 1988. Mechanical modeling of material damage. Journal of Applied Mechanics, Transactions ASME 55 (2), 280–286. Murakami, S., Hayakawa, K., Liu, Y., 1998. Damage evolution and damage surface of elastic–plastic-damage materials under multiaxial loading. International Journal of Damage Mechanics 7, 103–128. Nemat-Nasser, S., 1979. Decomposition of strain measures and their rates in ﬁnite deformation elastoplasticity. International Journal of Solids and Structures 15, 155–166. Nemat-Nasser, S., 1983. On ﬁnite plastic ﬂow of crystalline solids and geomaterials. International Journal of Applied Mechanics 50, 1114–1126. Nemat-Nasser, S., 1992. Phenomenological theories of elastoplasticity and strain localization at high strain rates. Applied Mechanics Reviews 45, S19–S45. Ortiz, M., 1985. A constitutive theory for the inelastic behavior of concrete. Mechanics of Materials 4 (1), 67–93. Pijaudier-Cabot, T.G.P., Bazant, Z.P., 1987. Nonlocal damage theory. ASCE Journal of Engineering Mechanics 113, 1512–1533. Rabotnov, YU.N., 1968. Creep rupture. In: Proceedings of the XII International Congress on Applied Mechanics. Stanford-Springer, pp. 342–349. Rousselier, G., 1987. Ductile fracture models and their potential in local approach of fracture. Nuclear Engineering and Design 105, 97–111. Seweryn, A., Mroz, Z., 1998. On the criterion of damage evolution for variable multiaxial stress states. International Journal of Solids and Structures 35, 1589–1616. Sidoroﬀ, F., 1981. Description of anisotiopic damage application to elasticity. In: IUTAM Colloquium on Physical Nonlinearities in Structural Analysis. Springer-Verlag, Berlin, pp. 237–244. Simo, J.C., Ju, J.W., 1989. Finite deformation damage-elastoplasticity: a non-conventional framework. International Journal of Computational Mechanics 5, 375–400. R.K. Abu Al-Rub, G.Z. Voyiadjis / International Journal of Solids and Structures 40 (2003) 2611–2643 2643 Simo, J.C., Honein, T., 1990. Variational formulation, discrete conservation laws, and path domain independent integrals for elasto– viscoplasticity. Journal of Applied Mechanics, Transactions of ASME 57, 488–497. Simo, J.C., Hughes, T.J.R., 1998. Computational inelasticity. In: Interdisciplinary Applied Mathematics. Springer, New York. Taylor, M.B., Zbib, H.M., Khaleel, M.A., 2002. Damage and size eﬀect during superplastic deformation. International Journal of Plasticity 18, 415–442. Thomason, P.F., 1990. Ductile Fracture of Metals. Pergamon Press, Oxford. Tvergaard, V., 1982. Material failure by void coalescence in localized shear bands. International Journal of Solids and Structures 18, 659–672. Tvergaard, V., Needleman, A., 1984. Analysis of cup-cone fracture in a round tensile bar. Acta Metallurgica 32, 57–169. Van Mier, J.G.M., 1984. Strain-softening of concrete under multiaxial loading condition, Ph.D. Thesis, Eindhoven. Venson, A.R., Voyiadjis, G.Z., 2001. Damage quantiﬁcation in metal matrix composites. Journal of Engineering Mechanics 127, 291– 298. Voyiadjis, G.Z., Kattan, P.I., 1992a. A plasticity-damage theory for large deformations of solids. Part I: Theoretical formulation. International Journal of Engineering Science 30, 1089–1108. Voyiadjis, G.Z., Kattan, P.I., 1992b. Finite strain plasticity and damage in constitutive modeling of metals with spin tensors. Applied Mechanics Reviews 45, S95–S109. Voyiadjis, G.Z., Kattan, P.I., 1999. Advances in Damage Mechanics: Metals and Metals Matrix Composites. Elsevier, Oxford. Voyiadjis, G.Z., Park, T., 1997. Local and interfacial damage analysis of metal matrix composites using ﬁnite element method. Engineering Fracture Mechanics 56 (4), 483–511. Voyiadjis, G.Z., Park, T., 1999. Kinematics description of damage for ﬁnite strain plasticity. International Journal of Engineering Science 37, 803–830. Voyiadjis, G.Z., Abu-Lebdeh, 1993. Damage model for concrete using bounding surface concept. Journal of Engineering Mechanics 119 (9), 1865–1885. Voyiadjis, G.Z., Deliktas, B., 2000. A coupled anisotropic damage model for the inelastic response of composite materials. Computer Methods in Applied Mechanics and Engineering 183, 159–199. Voyiadjis, G.Z., Deliktas, B., Aifantis, E.C., 2001. Multiscale analysis of multiple damage mechanics coupled with inelastic behavior of composite materials. Journal of Engineering Mechanics 127 (7), 636–645. Voyiadjis, G.Z., Venson, A.R., 1995. Experimental damage investigation of a SiC–Ti aluminide metal matrix composite. International Journal of Damage Mechanics 4, 338–361. Voyiadjis, G.Z., Abu Al-Rub, R.K., Palazotto, A.N., 2003. Non-local coupling of viscoplasticity and anisotropic viscodamage for impact problems using the gradient theory. Archives of Mechanics 55, 39–89. Voyiadjis, G.Z., Abu Al-Rub, R.K. Thermodynamic formulations for non-local coupling of viscoplasticity and anisotropic viscodamage for dynamic localization problems using gradient theory. International Journal of Plasticity, accepted for publication. Zbib, H.M, Aifantis, E.C., 1992. On the gradient-dependent theory of plasticity and shear banding. Acta Mechanica 92, 209–225. Zhu, Y.Y., Cescetto, S., 1995. Fully coupled elasto–visco-plastic damage theory for anisotropic materials. International Journal of Solids and Structures 32 (11), 1607–1641.